**HAL Id: pastel-00992073**

**https://pastel.archives-ouvertes.fr/pastel-00992073**

Submitted on 16 May 2014
**HAL is a multi-disciplinary open access**

archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Diffraction study of mechanical properties and residual**

**stresses resulting from surface processing of**

**polycrystalline materials.**

### Marianna Marciszko

**To cite this version:**

Marianna Marciszko. Diffraction study of mechanical properties and residual stresses resulting from surface processing of polycrystalline materials.. Other. Ecole nationale supérieure d’arts et métiers - ENSAM; AGH University of Science and Technology (Cracovie, Pologne), 2013. English. �NNT : 2013ENAM0037�. �pastel-00992073�

N°: 2009 ENAM XXXX

**Arts et Métiers ParisTech - Centre de Paris **
**AGH, University of Science and Technology, Krakow **

2013-ENAM-0037

### École doctorale n° 432 : Science des Métiers de l’ingénieur

*présentée et soutenue publiquement par *

**Marianna MARCISZKO **

11 octobre 2013
**Diffraction study of mechanical properties and **

**residual stresses resulting from surface processing **

**of polycrystalline materials**

**Doctorat ParisTech **

**T H È S E **

**pour obtenir le grade de docteur délivré par **

**l’École Nationale Supérieure d'Arts et Métiers **

**Spécialité “ Mécanique-Matériaux” **

Co-**Directeur de thèse μ Andrzej BACZMANSKI **
Co-Directeur **de la thèse μ Chedly BRAHAM **

**T **

**H **

**È **

**S **

**E **

**Jury**

**M. Wojciech LUZNY, **Professeur, WFIIS, AGH University of Science and Technology, Krakow Président

**M. Manuel FRANCOIS, **Professeur, LASMIS, Université de Technologie de Troyes Rapporteur

**Mme Malgorzata KAROLUS, **HDR, University of Silesia, Katowice Rapporteur

**M. Olivier CASTELNEAU, **HDR, PIMM, EcoleNationale Supérieure d’Arts et Métiers, Paris Examinateur

**M. Andrzej BACZMANSKI, **Professeur, WFIIS, AGH University of Science and Technology, Krakow Examinateur

**M. Chedly BRAHAM, **HDR, PIMM, EcoleNationale Supérieure d’Arts et Métiers, Paris Examinateur

**M. Krzysztof WIERZBANOWSKI, **Professeur, WFIIS, AGH,

### Acknowledgements

Foremost, I would like to thank my supervisors prof. Andrzej Baczmański and prof. Chedly Braham for providing me with the opportunity to complete my PhD thesis.

I especially want to thank prof. Andrzej Baczmański for his valuable guidance, scholarly inputs and consistent encouragement I received throughout the research work. I consider it as a great honor to have an opportunity to do my doctoral programme under his guidance and to learn from his research experience.

*Thank you Sir, for all your help and support. I could not have imagined having *
*a better supervisor and mentor. *

I would also like to thank Prof. Chedly Braham, for the academic support and the facilities provided to carry out the research work, for all his advices, discussions and suggestions.

The thesis would not have come to a successful completion, without the help I received from dr hab. Mirosław Wróbel and dr Wilfrid Seiler. I would like to express my special appreciation and gratitude to dr hab. Mirosław Wróbel for discussions, sample preparation, ideas and encouragement. I would like to thank dr. Wilfrid Seiler for assistance in carrying out experiments using X-ray diffraction and all valuable advises.

I am most grateful to prof. Krzysztof Wierzbanowski, prof. Olivier Castelnau and dr Sebastian Wroński for their kindness and support during my PhD studies.

I want to thank all members of the Group of Condensed Matter Physics (Faculty of Physics and Applied Computer Sciences, AGH, Kraków, Poland).

Last but not the least I would like to thank my family and my friends for their support and encouragement.

*I dedicate this thesis to my Mother, my Aunt, *
*Dorota and my beloved husband. Thank you for your *
*constant support and unconditional love. *

### T

### ABLE OF

### C

### ONTENTS

1. Introduction... 5

2. Strains and stresses measured by diffraction ... 9

2.1. Residual stresses and strains ... 9

2.2. Diffraction ... 14

2.3. Determination of stresses from diffraction data ... 23

2.3.1. Determination of first and second order stresses ... 24

2.3.2. Determination of third order strains and crystallite size ... 34

3. Methodology of stress measurements using X-rays ... 39

3.1. Methods with variable penetration depth ... 46

3.1.1. Standard geometries of stress measurement ... 46

3.1.2. Universal plot method ... 49

3.1.3. Scattering vector method ... 50

3.2. Methods with constant penetration depth ... 51

3.2.1. Multi-reflection grazing incidence X-ray diffraction ... 51

3.2.2. Multi-wavelength method ... 55

3.2.3. Multiple χ - method (pseudo-grazing) ... 55

3.3. X-ray diffraction elastic constants and stress factors ... 57

4. Aims of the Thesis ... 63

5. Tests, limits and experimental developments of the MGIXD method ... 65

5.1. Corrections of determined peak position ... 66

5.1.1. Intensity corrections ... 66

5.1.2. Peak shift due to refractive index smaller than 1 ... 69

5.2. Tests of the experimental configuration ... 82

5.2.1. Uncertainty of peak position ... 86

5.2.2. Testing incident beam optics ... 88

5.2.3. Influence of 2θ - zero position on the measured stress ... 91

5.2.4. Influence of z- position on the measured stress... 92

4

6. New interpretations of MGIXD measurements and verification of X-ray Stress Factors

(XSFs) ... 95

6.1. Self - consistent fitting of c/a parameter ... 95

6.2. Peak displacement caused by stacking faults ... 100

6.3. Verification of XSF used in MGIXD ... 104

6.3.1. Tensile test ... 105

6.3.2. Measurements of residual stresses ... 119

6.4. Conclusions ... 131

7. MGIXD method using different wavelengths of synchrotron radiation ... 133

7.1. X-ray measurements ... 134

7.2. Synchrotron measurements using MGIXD with different wavelengths and incident angles. ... 149

7.3. Energy dispersion measurement using synchrotron radiation... 177

7.4. Conclusions ... 181

8. General conclusions ... 183

List of publications published by author ... 187

5

### 1.

### I

### NTRODUCTION

The stress state is a characteristic parameter of the material state, together with the microstructure and the texture, it influences the material properties. That is why the stress analysis is of the great significance in industry and technology and became an important part of materials science. Progress in materials science and technology brought new challenges for stress analysis and various destructive and nondestructive methods have been developed.

Residual stresses are the stresses that remain after the original cause of the stresses (external forces, heat gradient) has been removed [1]. They can result from temperature or deformation gradients which are present in almost every step of material processing. Residual stresses can occur as a consequence of various technological treatments and manufacturing processes, but they can also arise in the component during its service life. Both the magnitude and the spatial distribution of residual stresses play key role in the behaviour of the material subjected either to heat treatment or plastic deformation. The strain - stress analysis is of particular utility for elucidating causes of failure. Depending on the orientation and value of the residual stresses superimposed by the external loads they can be unfavorable or beneficial for the component. The failure of a component in most cases starts in the near-surface area and occurs due to the initiation of plastic deformation or fracture when material is subjected to tensile loads. What is more all kinds of scratches, notches, etc. concentrate additional applied tensile stress near the surface which can cause the initiation of a crack. That is why; usually it is favorable with respect to the component lifetime to create compressive residual stresses in the near-surface area, which can stop fatigue crack propagation [2]. The basic mechanical surface treatments which allow gaining compressive residual stresses are deep-rolling and shot-peening [2, 3].

6

One of the ways to improve surface properties of the material are coatings. They can be beneficial in example for corrosion or wear resistance and can provide the long-term surface protection. The lifetime of a coating is strongly dependent on the residual stresses profile in the surface area.

Residual stresses influence the strength and fatigue behavior of the materials, but also they affect the chemical, electrical behavior of the thin films and can be very important in stress corrosion process [2, 3]. That is why residual stresses have to be taken into account while designing the structural parts especially in view of the improvement of their properties and increase of their lifetime. Stress analysis is important for constructions of and especially after various mechanical surface treatments. Studying the residual stresses of these materials is challenging issue due to depth gradients of micro and macro residual stresses and the influence of different parameters on their stability or relaxation. Consequently, reliable experimental methods for residual stress determination are of great practical importance. That is why diffraction method, which allow to separate micro- and macro-residual stresses and to study stress distribution in the sample are an indispensible tool. Despite great progress in stress analysis there are many questions which remain unsettled.

In the first part of this thesis (chapters 1-3), the diffraction methods of stress determination are introduced. The principles of lattice distortion, crystallite size and stress analysis based on the diffraction peak profile and measured lattice strain are described in chapter 2. Next, chapter 3 is devoted to a short characterization of different methodologies for stress determination using X-ray radiation (classical and synchrotron). The experimental methods are divided into two groups, i.e.: these in which the penetration depth of X-rays is constant or these for which penetration varies during measurement. On the basis of first three chapters the aims of the thesis are specified in chapter 4.

In chapters 5 – 7 the original results of this work, concerning development and testing of the multireflection grazing incidence X-ray diffraction (MGIXD) method for stress determination are presented. At first, the most important corrections of experimental data and tests of experimental setups are described (chapter 5).

In chapter 6 two important theoretical developments of the MGIXD method are
*presented. The first one enabling determination of c/a parameter and significantly *

7 improving quality of experimental data analysis for hexagonal structure has been proposed and tested. The second one in which density of stacking faults is taken into account is applied. What is more a verification of different types of X-ray stress factors (XSF), which can be applied to interpret the experimental data obtained using MGIXD method, is presented. Finally, examples of stress determination in surface layer for materials having high and low single crystal elastic constants anisotropy are shown.

In chapter 7 the methodology of data interpretation is developed in order to treat data obtained not only for different incident angles but also using simultaneously different wavelengths. It is shown that the new elaborated method is not only ‘multi-reflection’ but also ‘multi-wavelength’. Moreover, application of different wavelengths enables verification of the MGIXD measurements.

Chapter 8 concludes all the results presented in the thesis and formulates practical recommendations for the users of MGIXD method.

9

### 2.

### S

### TRAINS AND STRESSES MEASURED BY DIFFRACTION

The advantage of the diffraction method is its non-destructive character and the possibility of direct measurements of strains in precisely defined volumes of the material. Not only stresses can be determined from the diffraction methods. Intensities of the diffraction lines gives us the information about the crystallographic texture and the broadening of the diffraction lines allows to determine the size of the diffracting domains and the content of the crystalline defects such as dislocations and stacking faults [1]. Presence of stacking faults causes the diffraction peak shift and it depends on the probability of finding fault (Wagner 1966) [4].

The great need of precise stress determination has involved the introduction of new measuring methods and devices into experimental world. This progress would not have been possible without a detailed understanding of the theoretical principles of the used methodologies. In this work the diffraction methods of stress measurement will be used and developed. Because these methods are based on measurements of crystallographic lattice strains, the present chapter is devoted to explain how diffraction sees the strains caused by different kinds of stresses.

### 2.1.

### R

ESIDUAL STRESSES AND STRAINSAll solid materials are deformed when subjected to external loads. The deformation is manifested in displacement of points in the body under load from their initial positions. When a body underlies certain stresses, the strain response depends on the elastic properties of the material. The strain can be of elastic and of plastic kind. As long as the forces acting on the body are below a certain limit, the deformation is reversible and is called elastic deformation. For this kind of deformation, when the load is removed the displacements vanish and the body returns to its unloaded configuration. However, when

10

the forces acting on the material are higher than the limit, the material undergoes plastic deformation. In this case some permanent deformation remains after the load is removed. If the deformation of the material is homogeneous the deformation of all points of the body is the same. However, when the deformation varies from point to point along any direction in the material volume, the deformation distribution is considered heterogeneous [1, 3].

The relation between the stresses and elastic strain tensor for elastic body is given by generalized Hooke’s law [1]:

or (2.1)

where: and are the components of stress and elastic strain tensors, while ( ) are the components of stiffness (compliance) tensor.

The stress component σij is defined to be the force per area acting on the i-face in

direction j (Fig. 2.1).The σii components for which i-forces are normal to the i-faces are

called normal components, and the σij components (where i≠j) for which j-forces are

parallel to the i-faces are called shear components. Stresses form a 9 component symmetrical 2nd rank tensor which can be written in the matrix notation [1]:

11 12 13
21 22 23
31 32 33
*ij*
σ σ σ
σ σ σ σ
σ σ σ
=_{} _{}
(2.2)

Fig. 2.1. Orientations of stress tensor components with respect to definition surfaces

*ij* *cijkl* *kl*

σ = ε ε*kl* =*sklij*σ*ij*

*ij*

11 In static conditions, the principle of conservation of angular momentum implies that σij = σji and only 6 of the 9 components are independent [1].

The external forces acting on the material causes the deformation which can be described by the strain tensor:

11 12 13
21 22 23
31 32 33
*ij*
ε ε ε
ε ε ε ε
ε ε ε
=_{} _{}
(2.3)
where:
0 0 0
1

lim lim lim

2
*i* *i* *j*
*j*
*i* *i*
*ii* *ij*
*x* *x* *x*
*i* *i* *j*
*v*
*w* *v*
*and* *for* *i* *j*
*x* *x* *x*
δ δ δ
δ
δ δ
ε ε
δ δ δ
→ → →
= = _{} + _{} ≠

while i, j = 1, 2, 3 (the displacements for two dimentions are defined in Fig. 2.2).

Fig. 2.2. Displacement of the body used in strain definition.

The proportionality constants cijkl in Eq 2.1 describe physical property of the elastic

substance under load. The cijkl tensor relating strains and stresses (Eq. 2.1) is a 4-th rank

tensor of elastic stiffnesses, and it has 81 components. Because of stress and strain symmetries it is possible to reduce the number of the components to 36 independent ones. In the case of monocrystal this number furthermore can be reduced taking into consideration the symmetry of the crystal lattice [1]. For isotropic body the cijkl constants

depend only on two parameters (E – Young’s modulus and Poisson's ratio), and they do not change with direction in the body. However, for anisotropic materials these properties vary with orientation and more elastic constants are needed to describe elastic properties [3].

12

By definition, the residual stresses are self-equilibrated stresses [2]. The residual stresses must fulfill the equilibrium condition in each point of the material [2, 3]:

(2.4)

And surface condition:

i.e. σ* _{ij}*⋅ =

*n*0 (2.5)

_{i}where is the normal versor to sample surface.

When flat samples are taken into consideration the ‘plane stress’ condition can be assumed. It is possible due to their small expansion in one direction (e.g., x3) as compared

to the other two directions, so often stresses in the x3-direction can be assumed to be

negligible (σ13= σ23 = σ33 = 0). The stress equilibrium conditions imply that tensile residual

stresses in a certain direction within one part of a body are always balanced by matching compressive residual stresses in another part. Thus, the residual stress state of a component can never be expressed by a single residual stress tensor, but only by residual stress distribution. This also implies the presence of residual stress gradients. Strong residual stress gradients are often present in the near-surface area of components, due to surface treatment, or because the residual stress component normal to the surface needs to vanish but stress continuity has to be observed in the bulk material [2].

Due to granular structure of polycrystalline aggregates, the stress and strain states in these materials should be considered and described at different scale. It is possible to distinguish residual stresses of Ist type (macrostresses) and IInd type, IIIrd type (microstresses). The residual stress distribution in a material is the sum of type I, type II, and type III residual stresses:

( )*r* *I* *II* *III*( )*r*

### σ

= +### σ σ σ

+ (2.6)(2.7)

*where: Vtot is the total volume of the sample and describes position. *

0
*ij*
*i*
*x*
σ
∂
=
∂
0
*n*
σ ⋅ =
*n*
( ) 0
*tot*
*V*
*r dV*
σ =

### ∫

*r*

13
Type I residual stresses σ*I* represent the average residual stresses acting within all
phases and crystallites in the gauge volume Vga. These stresses are defined by mean value

*over volume of considered part of the sample (Vga*, for example gauge volume in

diffraction experiment), i.e.:

1
( )
*ga*
*I*
*ga V*
*r dV*
*V*
σ =

_{∫}

σ (2.8)
The gauge must be large enough to represent macroscopic material containing a sufficient number of crystallites and all phases present in the material.

Type I residual stresses (or first order) result from long range strain incompatibilities introduced, e.g., by strain or temperature gradients in a manufacturing process. The distribution and magnitude of type I residual stresses often can be controlled by modifying the process parameters of a production process [2].

Type II residual stresses (σ*II*, second order) describe the mean deviation from the
macroscopic residual stress level σ*I* calculated over the volume of individual
*polycrystalline grain (Vgr*), i.e.:

1
[ ( ) ]
*gr*
*II* *I*
*gr V*
*r* *dV*
*V*
σ =

_{∫}

σ −σ (2.9)
In a multiphase material type II residual stresses (or second order) are taken as the volume
weighted average residual stresses σα calculated over the volume of crystallites belonging
*to a phase α (Vα*) or as the average residual stresses for those crystallites of the phase α

which contribute to the measurement:

1
[ ( ) *I*]
*V*
*r* *dV*
*V*
α
α
α
σ =

_{∫}

σ −σ (2.10)
Type II residual stresses arise for instance due to deformation misfits between neighboring grains and due to temperature or deformation induced misfits between different phases in a multiphase material [2].

Type III residual stresses represent the local deviation of the residual stresses within an individual crystallite from its average residual stresses in the grain

( )
*III*

*r*

14

(variation on the atomic scale). Thus, the average type III residual stresses does not result in macroscopic distortions. Type III residual stresses are caused, e.g., by voids, solute atoms, or dislocations in the crystal lattice [1, 2].

The all three types are present, for example, in mechanically machined samples. The microstructure of materials subjected to plastic deformation changes significantly. Due to twinning mechanism and slips occurring on the crystallographic planes plastic deformation of the grain occurs. In general, this irreversible deformation it is slightly different for neighboring grains, which leads to compression or stretching of single grains. This mechanism is a primary source of internal second order stresses. In addition, during the plastic deformation, a large amount of point defects and dislocations is generated. The latter phenomena lead to creation of internal stress fields. Accumulation of dislocation inside the grains produces the third order stresses.

Each type of stresses existing in material influences crystallographic lattice causing its distortion. The first and second order stresses cause mean elastic lattice strains for particular polycrystalline grains. The third order stresses leads to distortion and strain heterogeneity within grains. Both effects can be seen in diffraction experiment as the shift and broadening of the diffraction peaks. To present methods for strain measurement, at first the diffraction phenomenon must be described.

### 2.2.

### D

IFFRACTIONDiffraction on crystallographic lattice is associated with certain phase relationships between waves scattered in all directions by the atoms. The phases of the scattered rays are relatively shifted in the most of directions. However, in some particular directions the reflected waves exhibit the same phase and due to constructive interference they are strengthened, creating a diffracted beam.

In order to describe the diffraction phenomenon using kinematic theory, crystal can be treated as a periodic arrangement of atomic planes, which act like a mirror for the incident radiation [5]. The incident beam strikes the crystallographic planes at an angle

*θ and it is reflected from them also at an angle θ (see Fig. 2.3b). Therefore, the total angle *

15
*equal to ‘d’ the difference of the paths for the rays reflected from these planes is equal to *
*2d sinθ (Fig. 2.3a). Constructive interference will occur when the waves have the same *
*phase, so when the path difference between them will be equal to an integer multiples (m) *
*of the wavelength (λ), so when the equation: *

2 sin

*m*

### λ

=*d*

### θ

(2.11)is fulfilled. The above equation is called Bragg’s law [1] and it is a basic geometrical diffraction condition.

Fig. 2.3. Difference between paths of the beams reflected from neighboring crystallographic planes (a) and construction of the scattering vector (b), where and denotes wave vectors for the incident and diffracted beams, respectively.

Bragg’s equation can be expressed also in an equivalent way. Let us denote by a wave

vector of the incident beam and by a wave vector of diffracted beam. Diffraction vector

can be defined as: and it is perpendicular to the plane of reflection (Fig2.3 b). The length of the diffraction vector is given by:

(2.12)
*i*
*k* *kd*
*i*
*k*
*d*
*k*
*d* *i*
*k* *k* *k*
∆ = −
4 sin
*d* *i*
*k* *k* *k* π θ
λ
∆ = − =

16

Considering Bragg’s law, the above equation can be rewritten as:

(2.13)

*where: hkl are the indices of reflection which for the first order reflection (i.e., for the *
*lowest hkl and m=1 in Bragg’ law) are equal to Miller indices of the of the reflecting *
*planes, while for the m-th order of reflections * *=d/m where d is the interplanar space. *

Because (where is the reciprocal lattice vector), so the general condition

for the occurrence of diffraction (when both vectors and have the same orientations, i.e., they are perpendicular to the reflecting plane) can be written as:

(2.14)

*Expressing the * vector by primitive translation vectors of the reciprocal lattice

and multiplying both sides of Eq. (2.14) by primitive translation vectors (where the latter basis vectors are defined for the real lattice) the Laue equations can be obtained [7]:

and (2.15)

*The Miller indices of crystallographic plane in the real space (h,k,l) correspond to *
the coordinates of lattice point in the reciprocal space.

Bragg or Laue equations give the geometrical condition of the diffraction; however,
they do not contain the information about the intensity of the diffracted beam. The
intensity will depend on the kind of the diffracting atoms and their arrangement in the unit
cell. In the case of X-ray diffraction electrons are responsible for coherent scattering of the
electro-magnetic wave. During the diffraction each of the electrons in the atom scatters
elastically part of the incident beam. In order to describe the ability of diffraction for each
*atom the atomic factor f depending on the Z (atomic number) of the element is used [8]. In *
the direction of diffraction, specified by the Bragg condition, the ability of diffraction by
*the unit cell is described using the structural factor Fhkl*. The complex value of this factor is

2
*hkl*
*k*
*d*
π
∆ =
*hkl*
*d*
2
*hkl*
*hkl*
*d*
*G*
π
= *Ghkl*
*k*
∆ *Ghkl*
*hkl*
*k* *G*
∆ =
*hkl*
*G*
1 2 3
*hkl*
*G* =*hb* +*kb* +*lb*
1, 2, 3
*a a a*
1 2
*a k*∆ = π*h* *a*_{2}∆ =*k* 2π*k* *a*_{3}∆ =*k* 2π*l*

17
calculated as a sum of the amplitudes of the coherently diffracted rays from the atoms in
*the unit cell (assuming unit amplitude of the incident beam) [8]. For unit cell having M *
*atoms at positions described with the coordinates (xn, yn, zn*), the structural factor can be

expressed as [6]:

(2.16)

*where: hkl are the indices of considered reflection, fn is the atomic factor of the n-th atom *

*and M denotes number of atoms in unit cell *

The intensity of the beam diffracted from all the atoms in the unit cell in the
direction described with the Braggs law is proportional to the square of the amplitude of
*the resultant beam, and consequently, it is proportional to | Fhkl* |2. The above equation

*allows calculating the intensity of each hkl reflection when the atomic positions are known. *
Analyzing intensities of the beams diffracted on different plains (i.e., knowing the values
*of | Fhkl* |2 from experiment) the arrangement of the atoms in unit cell can be refined. In this

aim the numerical Rietveld method can be used [9].

In description of diffraction experiment it should be remembered that the crystals are not ideal and the incident beam is not strictly parallel and monochromatic. The actual X-ray beam contains rays divergent and convergent as well as parallel, so the intensity of diffracted beam will be registered not only for the Bragg angle but also in same small range around this angle. This effect is known as the instrumental broadening of registered diffraction peak. Also, the microstructure of the material significantly influences the profile of the measured peak, i.e. the broadening of the peak is affected by the size of diffracting crystal and its real internal structure containing defects of the lattice.

*To explain the role of finite crystal size the ideal crystallite having N points (equal to *
*number of unit cells) can be considered. The positions of n-th point of the real lattice can *
be defined by the vector:

(2.17)

where: * are the basis translation vectors and m1, m2 , m3* are the integer or zero

numbers.
2 ( )
1
*n* *n* *n*
*M*
*i hx* *ky* *lz*
*hkl* *n*
*n*

*F*

*f e*

π + +
=
### =

### ∑

1 1 2 2 3 3*n*

*m a*

*m a*

*m a*ρ = + + 1, 2, 3

*a a a*

18

Next, the diffraction vector can be expressed as the linear combination of the basis vectors in reciprocal space:

(2.18)

*where h1, h2, h3* are the vector coordinates given by real values. These values are chosen

*close to the point of reciprocal lattice corresponding to the considered reflection hkl, *
*i.e. h1=h, h2=k, h3=l when Eq. 2.14 is fulfilled and * determines the position of the

reciprocal lattice point.

If the point of the observation (detector counting intensity of diffracted beam) is far
away from the crystal the phase difference of the waves from two scattering centers is
equal: . Assuming amplitude of incident beam equal to unity, the amplitude
*An* of the wave diffracted on a lattice point (representing unit cell) in the position can be

expressed as :

**(2.19) **

*where Fhkl* stands for an amplitude of the beam diffracted on the unit cell which is equal to

*the structural factor defined by Eq. 2.16 and Ae* is an amplitude of wave scattered by one

electron. In order to gain the amplitude from all scattering centers it is necessary to sum up over all lattice points [:

**(2.20) **

Following the calculations given by for example Kittel [10], the dependence of diffracted intensity on the length and direction of scattering vector ( ) can be derived: 2 2 2 2 2 3 3 1 1 2 2 1 2 3 2 2 2 1 2 3 sin sin sin ( , , )

sin sin sin

*total* *e* *hkl*
*N h*
*N h* *N h*
*I h h h* *A* *A F*
*h* *h* *h*
π
π π
π π π
= = (2.21)

*where: N1, N2 and N3* are the numbers of real lattice point in directions of , and

*N= N1 N2 N3*.
*k*
∆
1 1 2 2 3 3
*k* *h b* *h b* *h b*
∆ = + +
*k*
∆
*k*
∆
*n* *k* *n*
φ ρ
∆ = ∆
ρ
exp[ ] exp[ ]
*n* *e* *hkl* *n* *e* *hkl* *n*
*A* = *A F* − ∆*i* φ = *A F* − ∆*i k*ρ
exp
*N*
*total* *e* *hkl* *n*
*n*
*A* = *A F*

### ∑

_{}− ∆

*i*ρ

*k*

_{}1 1 2 2 3 3

*k*

*h b*

*h b*

*h b*∆ = + + 1, 2

*a a*

*a*

_{3}

19
Integrating the above equation around point of reciprocal lattice
(e.g. the total diffracted intensity proportional to the number of
*unit cells (N) can be calculated, i.e.: *

** (2.22) **

To see the intensity distribution around given point in reciprocal lattice the
*particular reflection 00l can be considered. If we follow the intensity variation only in the *
direction of vector we can put and in Eq.2.21, i.e.:

(2.23)

Using Eqs. 2.12, 2.13 and 2.18 the value of *can be related with 2θ angle: *

**(2.24) **

In Fig.2.4 the one dimensional function vs. * for l=1 is shown. Also, this *

*function vs. 2θ is presented assuming * = =1Ǻ. The calculation were performed for
=500 and =1000 atoms (or crystallographic planes) in the direction along the
scattering vector. This situation corresponds to the crystallite size of 50 nm and 100 nm
along the direction of scattering vector.

Fig. 2.4. Function vs. * (for l=1) and the same function vs. 2θ *

(assuming = =1A) are shown.

1 2 3
*hkl*
*k* *G* *hb* *kb* *lb*
∆ = = + +
1/ 2 1/2 1/ 2
2 2 2
1 2 3 1 2 3 1 2 3
1/ 2 1/ 2 1/ 2
( ) ( , , )
*h* *k* *l*
*tot* *N* *e* *hkl* *e* *hkl*
*h* *k* *l*
*I* *hkl* *I h h h dh dh dh* *A* *A F* *N N N* *A F* *N*
+ + +
− − −
=

_{∫ ∫ ∫}

= = =
3
*b*

*h*

_{1}=0

*h*

_{2}=0 2 2

_{2}

_{2}3 3 3 1 2 2 3 sin ( ) sin

*e*

*hkl*

*N h*

*I h*

*A F*

*N N*

*h*π π = 3

*h*00 3 2 sin

*l*

*d*

*h*θ λ = 2 3 3 2 3 sin sin

*N h*

*h*π π

*h*3

*00l*

*d*

### λ

3*N*

*N*

_{3}h

_{3}0.996 0.997 0.998 0.999 1.000 1.001 1.002 1.003 1.004 0.0 2.0e+5 4.0e+5 6.0e+5 8.0e+5 1.0e+6 1.2e+6 N3=500 N3=1000 2θ (o) 59.8 59.9 60.0 60.1 60.2 0.0 2.0e+5 4.0e+5 6.0e+5 8.0e+5 1.0e+6 1.2e+6 N3=500 N3=1000 2 3 3 2 3 sin sin

*N h*

*h*π π

*h*3

*00l*

*d*

### λ

20

The following conclusion can be drawn from the above equations illustrated in Fig. 2.4:

• *intensity at the point of reciprocal lattice (or for 2θ0* angle which fulfill strictly

Bragg low) is proportional to the square from numbers of reflecting planes being

perpendicular to the scattering vector (

3
2
2
3 3
3
2
0
3
sin
lim
sin
*h*
*N h*
*N*
*h*
π
π
→ = ),

• broadening of intensity given by width of the peak is proportional to 1/ ,
i.e. number of reflecting planes in the direction of scattering vector _{, }

• total (integrated) intensity is proportional to _{, }

• broadening of the intensity around the point of reciprocal does not depend on the
*reflection order (the same profile of peak be obtained for different l, because the *
*period of function defined in Eq. 2.23 with respect to h3* is equal to1).

*The above conclusions can be generalized for any hkl reflection. *

More general derivation of the intensity distribution in the diffraction peak for
crystallites with lattice distortion was given by Warren and Averbach [11]. In this case also
the partial waves diffracted on scattering centres are considered but the calculations were
performed for a powder sample and contributions of diffracted intensity from grains having
different orientations was integrated. Moreover, the scattering centres are shifted from the
points of nets. The result of calculations is given as the Fourier series (presented also for
*the 00l reflection): *

(2.25)

*which can be also written with respect to 2θ angle substituting * by relation 2.24. The
coefficients of expansion are [11]:

(2.26 a) and ** (2.26 b) **

where and < > are the square mean and mean values of the lattice microstrains in the direction of scattering vector, inside a crystallite (those which are caused by defects

3
*N*
*k*
∆
3
*N*
2
3 3 3
( ) *e* *hkl* [ *n*sin(2 ) ' cos(2*n* )]
*n*
*I h* = *A F* *N*

### ∑

*a*π

*nh*+

*a*π

*nh*3

*h*

### (

2 2 2 2### )

1 2− π*n l*<ε >

*B*

*n*

*n*

*a = a*

*a*'

*= −*

_{n}*a*

_{n}B### (

2π2*n l*2 2 < >ε

### )

2 ε < > ε21 and associated with the third order stresses), and is the factor depending on the crystallite size (also in the direction of scattering vector).

The coefficients represent nonsymmetrical distribution of strains within the crystallite. However, if we consider only effect of the third order stresses and the distribution of defects is random (or in more general case if the probability of and -occurrence is equal) the coefficients vanish.

It is clear that, the coefficients bring an important information about size of
crystallite ( ) and square mean strain of its lattice strains caused by the third order
stresses. The * factors do not depend on the order of reflection (00l), and it can be shown *
[11] that:

(2.27)

where is an average number of reflecting plains along scattering vector.

On the other hand the function of vs. depend the order of reflection
*(00l). Therefore the analysis of size and strain by Warren-Averbach is based on the *
expansion of diffraction peak profile into a Fourier series and then calculation of

and (or rather , i.e., size of crystallite) in direction of scattering vector from
*An* coefficients. In this method two diffraction peak must be measured for two orders of

**reflections (usually the first and second order for example 111 and 222). **

Next step in analisis of peakprofile, after single crystal and powder sample is it the case of polycrystalline aggregate which is built from crystallites having different orientations (like in powder but often some orientations are preferred in the case of crystallographical texture). Moreover, in real structure of polycrystalline material mosaic microstructures of grains can have a significant impact on diffraction (especially after large plastic deformation). Such a crystal do not have atoms arranged in a perfectly regular network, but a large number of small blocks, each of which is slightly disoriented with respect to its neighbors [6]. Diffraction peak results from the coherent scattering of the incident beam on the so-called domains which in fact represent crystallites considered by

*B*
*n*
*a*
'_{n}*a*
ε ε
'_{n}*a*
*n*
*a*
*B*
*n*
*a*
*n*
*a*
3
0
1
*n*
*d*
*dn* _{→} = −*N*
*B*
*n*
*a*
3
*N*
*n*
*a* <ε2 >
2
ε
< >
3
*N* *D*=*N a*3 3

22

Warren and Averbach [11, 12]. The size of such domains is of tents or hundreds nanometres, so their effect on the peak broadening is comparable with that shown in Fig. 2.4. In the case of polycrystalline material usually the same methods of profile analysis are used as for powder sample, however, in this case such properties as crystallographic texture, complex microstructure and moreover presence of residual stresses should be considered in interpretation of the obtained results.

The polycrystalline grains are not free as in the powder sample but they interact elastically with their neighbours. Therefore, the first and second order stresses causing mean elastic deformation of the lattice which can be observed as a shift of the diffraction peak position. Using diffraction methods the mean lattice strain can be determined as the relative change of interplanar spacing and can be calculated from the relative shift of the peak:

(2.28)

or using Bragg’s relation (Eq. 2.11):

(2.29)

where *is the mean interplanar spacing for {hkl} crystallographic planes *

determined in the studied sample, is interplanar spacing for these planes but in stress
free crystallite, 2( ) is a shift of diffraction peak with respect to the position in
*stress free material (2θ0*).

It should be underlined that the <...>*{hkl}* is the volume of the crystallites (in fact

domains in polycrystalline grains) which take part in diffraction, i.e., they have such lattice
orientations for which the scattering vector _{ is perpendicular to symmetrically }
*equivalent {hkl} planes (or strictly: as close to the normal as diffracted intensity appears), *
see Fig. 2.5. Therefore, diffraction gives us information about average lattice strains for
group of grains, but not directly about stress in particular grain. Further analysis is
necessary to relate these strains with stress of Ist and IInd type [13, 14]. Also it should be
mentioned, that the <...>*{hkl}* average is calculated over different grains exhibiting different

strains (due to different lattice orientations or second order stresses), thus their contribution

0
{ } { }
{ } 0
{ }
*hkl* *hkl*
*hkl*
*hkl*
*d* *d*
*d*
ε < > −
< > =

### (

### )

{*hkl*} cot 0 {

*hkl*} 0 ε θ θ θ < > = − < > − {

*hkl*}

*d*< > 0 {

*hkl*}

*d*{

*hkl*} 0 θ θ < > −

*k*∆

23 in diffraction peak cause additional broadening (however in most cases much smaller than this produced by the third order stresses).

Fig. 2.5. The selective character of diffraction. Only the grains for which the scattering vector is normal to the reflecting planes {hkl} and Bragg’s law is fulfilled contribute to diffracted intensity.

Concluding it should be underlined that the peak broadening of the diffraction peak measured for polycrystalline material brings an important information about the size of so called coherent domain and mean square internal strains (caused by defects and third order stresses), while the shift of diffraction peak can be related to mean lattice strains caused by the external or residual stresses acting on the grains embedded in polycrystalline aggregate (caused both by the first and the second order stresses). In the next chapters the method for extracting such information from experimental data will be shown.

### 2.3.

### D

ETERMINATION OF STRESSES FROM DIFFRACTION DATAThe residual stress state analysis is based on the diffraction measurements of the
interplanar spacings in different directions of the scattering vector [1]. In order to
describe the geometry of measurements it is necessary to introduce two coordinate
**systems: the coordinate system connected with the specimen (S) and the coordinate system *** connected with the scattering vector. The latter frame is called the laboratory system L, *
because scattering vector is often fixed with respect to laboratory and sample is rotated
(e.g. Eulerian cradle). These systems are defined as follows (Fig. 2.6):

* The specimen reference system (S): The S*3 axis is orientated perpendicular to the specimen

*surface. Axes S1 and S2* lie in the surface plane. If a preferred direction within the plane of

*the surface exists, e.g. the rolling direction, the S1* direction is usually orientated along this

preferred direction.
*k*
∆
2
ε
< >
*k*
∆

24

* The laboratory reference system (L): L3* axis coincides with the diffraction vector , and

*L2* axis lies in the surface plane.

* Then the orientations so defined L system with respect to S system can be described *
by two angles ψ and φ defined in Fig. 2.6, i.e. ψ

*is between S3 and L3*axes, while φ is

*between L3* and its projection on the sample surface. These angles also determine

orientation of the scattering vector ∆*k L*|| _{3}.

Fig.2.6. Orientation of the scattering vector with
* respect to the sample system S. The *ψ and φ

**angles define the orientation of the L system (the***L2*axis lies in the plane of the sample surface).

* Additionally, η – rotation of the L system around *
scattering vector is shown (this rotation will be
used I the scattering vector method, section
3.1.3).

*2.3.1.DETERMINATION OF FIRST AND SECOND ORDER STRESSES*

To analyse first order stresses, the mean lattice strains has to be determined from measured
shifts of the diffraction peak (Eqs. 2.28 or 2.29). Because the exact position of the
diffraction peak must be determined with high accuracy it is necessary to take into account
phenomena influencing the profile [1, 6] or position of the peak. To do this the following
*depending on 2θ factors are introduced in strain analyses: *

• *Lorentz-polarization factor - LP(2θ), *

• *absorption factor - Ab(2θ), *

• *refraction factor (in the case of small incidence angles) – R(2θ). *

*Usually, the dependence of atomic factor fn* (see Eq. 2.15) and temperature factor do

not significantly influence peak profile, and they are not taken into account in corrections.
*The LP(2θ), Ab(2θ) factors are described in Culity [6] or Noyan [3], while the R(2θ) factor *
is in detail considered in this work.

*k*

25
Also, the asymmetry of the background may be an imortant problem in the peak
position determination. In order to make the correction for the background it is necessary
*to apply function Ibcg(2θ) which can be obtained by fitting a low degree polynomial *

function (usually simply linear function) to the background intensities on both left and
right hand sides of the diffraction peak [1]. To introduce all corrections the background
*must be subtracted from the measured intensities, the result must be divided by LP(2θ) and *
*Ab(2θ) factors for every 2θ angle and next peak must be shifted by the - 2θR* angle (in the

case of small angle of incident beam), i.e.:

(2.30)

*where the Iexp(2θ) and Icor(2θ) are the experimental and corrected intensities, respectively. *

After correction and proper preparation of data the precise position of the interference-peak can be determined calculating center of gravity of the peak or fitting theoretical functions to the intensity profile (e.g.: Gauss, Person VII, Lorentz or Pseudo-Voigt functions) [1]. Although the displacement of the diffraction peak is generally small, the fitting procedures with, e.g., Lorentz, Gauss or Voigt functions allow to determine a very precise position of the peak.

Centre-of-gravity method. In this method the intensities of Kα1-Kα2 lines are averaged out

in the result. The peak position is calculated by [1]:

(2.31)

Usually the integration is performed over some threshold value assumed relatively to the
maximum peak-intensity.
exp(2 ) (2 )
(2 2 )
(2 ) (2 )
*bcg*
*cor* *R*
*I* *I*
*I*
*LP* *Ab*
θ θ
θ θ
θ θ
−
− =
(2 )2 2
2
(2 ) 2
*c g*
*I* *d*
*I* *d*
θ θ θ
θ
θ θ
< >=

### ∫

### ∫

26

Fitting of the Gauss function. In this method the diffraction peak is fitted by [9]:

**(2.32) **

where: and *, w is the full width at half maximum (FWHM *

defined as the full angular width at half-maximum intensity of the diffraction peak [1]),

related with integral breath by equation: (β is defined as the ratio of the peak

area to the peak maximum [1]).

Fitting of the Lorentz function [9]:

(2.33)

where: , * and w can be related with β by equation: *

For better resolution of determined position it is recommended to use Pearson VII-functions or Voigt-VII-functions instead of Gaussian or Lorentz distributions. Those VII-functions are much more flexible in describing the peak profile and fits better to the measured intensities [1].

The Pearson VII-function is given by [9]:

(2.34)

where: , , Γ(m)=(m-1)!, and m is the shape

parameter.
2
max
(2 ) exp (2 2 )
*G* *G* *G*
*I* θ =*a* _{}−*b* θ− θ _{}
2 ln 2
*G*
*a*
*w* π
= 2
4 ln 2
*G*
*b*
*w*
=
2 ln 2
*G*
*w* π
β =
2
max
(2 )
1 (2 2 )
*L*
*L*
*L*
*a*
*I*
*b*
θ
θ θ
=
+ −
2
*L*
*a*
*w*
π
= *bL* 4_{2}
*w*
=
2
*L*
*w*
π
β =
2
max
(2 )
1 (2 2 )
*VII*
*VII*
*P* *m*
*VII*
*a*
*I*
*b*
θ
θ θ
=
_{+} _{−}
1
( ) 2 2 1
1
( )
2
*m*
*VII*
*m*
*a*
*w*
*m* π
Γ −
=
Γ −
1
2
4 2*m* 1
*VII*
*b*
*w*
−
=

27 The Pseudo-Voigt function [15, 16, 17] is superposition of Gaussian (G’) and Lorentzian (L’) functions, given by the expression [9, 17]:

(2.35)

where: η is the relative contribution of Gaussian component.

If Lorentzian and Gauss components are normalized than pseudo-Voigt is also normalized.

It should be stated that from X-ray diffraction experiments performed on laboratory diffractometers (it is not the case of synchrotron radiation) the intensity of the incident beam is composed from two emission lines Kα1 and Kα2 exhibiting very similar

wavelengths. The contribution of both lines cannot be experimentally separated totally and it has to be done at the stage of data analysis using one of two possible methods:

• influence of Kα2 intensity can be removed using Rachinger method [18] assuming

theoretical ratios of intensities I(K α1)/I(K α2)=0.5 and knowing difference between

wavelengths λKα1 and λKα1.Next, the center of gravity is calculated for one peak or

peak profile is fitted by above defined functions,

• doublet of two measured is treated together: o superposition of defined above functions:

(2.36)

is fitted to experimental points (where is the distance between two peaks resulting from two lines for given theoretical difference of wavelengths 2λKα1 and 2λKα1) ratio I (K α1)/ I (K α2)=0.5 is assumed,

o or the centre of gravity is calculated for the doublet but mean next mean wavelength must be used in Bragg’s law, i.e.: λmean=(2λKα1+λKα2)/3

In Fig. 2.7 examples of peak position determination were presented. Peaks were measured for Al powder using Kα Cu radiation (λKα1=1.54056 Å and λKα2=1.54433Å) on

PANalytical - X’Pert MRD diffractometer (AGH, Kraków) with Göbel mirror using

' '
m ax m ax
( 2 ) ( 2 2 ) (1 ) ( 2 2 )
*p V*
*I* θ =η*L* θ − θ + −η *G* θ − θ
1 1 1 2
(2 ) * _{K}* (2 ) 0.5

*(2 2*

_{K}

_{K}*)*

_{K}*I*θ =

*I*

_{α}θ +

*I*

_{α}θ− θ

_{α}

_{−}

_{α}1 2 2θ

_{K}_{α}

_{−}

_{K}_{α}

28

parallel beam configuration, described in Table 5.4 (chapter 5). Different peak broadenings are seen and high accuracy of measured peak position were obtained when doublet Kα1 and

Kα2 (two peaks) was fitted using the pseudo-Voigt function.

a) b)

c) d)

Fig. 2.7. Examples of different methods for position determination: calculation of center of gravity (a), and fitting of Gauss (b), Lorentz (c), pseudo-Voigt (d) functions. Experimental peak was measured for Al powder using PANalytical - X’Pert MRD diffractometer (AGH, Kraków - configuration given in Table 5.4.).

Table 2.1. Comparison of the determined positions for Al powder using 4 different methods. Fitting position 2θ (°) Pseudo-Voigt 65.1000a ± 0.0003 Lorentz 65.0982a ± 0.0002 Gauss 65.1007a ± 0.0002 center of gravity 65.1023a (65.1620b)

29
When the positions of diffraction peaks are determined the stress analysis can be
performed. The diffraction strain * measured along L3* direction (see Eq. 2.28

and Fig. 2.6) are defined as the average strain over diffracted grains volume (Fig. 2.5) which is calculated as [19, 20]:

(2.37)

where * is the strain along L3 direction for (hkl) plane, ψ and * are the

*angles describing the orientation of the diffraction vector (along L3*) ith the respect to the

*specimen reference system, ξ – the rotation around the diffraction vector (see Fig. 2.8), *
is the function representing crystallographic texture, i.e. orientation
distribution function ODF (defined in [21]) expressed in terms of measurement parameters
*and the rotation angle ξ. Summation * *is over all symmetrically equivalent planes {hkl}. *

Fig. 2.8. Definition of lattice rotation around the scattering vector normal to (hkl) plane.

In the above average only the criterion for selection of grain orientations is considered, but also the average must be calculated over the gauge volume using weight of the intensity scattered by different grains (accounting for absorption).

{ }
( , *hkl*
ε φ ψ
< >
2
33
{ _{} 0}
{ } 2
{ _{} 0}
( , , , ) ( , , , )
( , )
( , , , )
*L*
*hkl*
*hkl*
*hkl*
*hkl* *f hkl* *d*
*f hkl* *d*
π
π
ε ξ φ ψ ξ φ ψ ξ
ε φ ψ
ξ φ ψ ξ
< > =

### ∑ ∫

### ∑ ∫

33( , , , )*L*

*hkl*ε ξ φ ψ φ ( , , , )

*f hkl*ξ φ ψ {

*hkl*}

### ∑

*k*∆

30

For polycrystal composed of elastically isotropic crystallites (for example tungsten) Hooke’s law [19] can be applied to relate the macrostrains with the first order stresses:

(2.38)

where: and are the first order stresses and strains (mean over whole diffraction

gauge volume), and * are crystal compliances (equal for isotropic material), S1* and

*S2are the only independent components of Sijkl* for elastically isotropic specimen and is

**the Kroneckers delta (all tensors are defined in S system). **

In this case the elastic strain tensor is identical for all crystallites and also for diffracting group of grains [19]:

(2.39)

**where L superscript means that the strain is expressed in L system (tensor in S system have ****not additional superscripts as in Eq. 2.38). **

Then it is possible to calculate ** (L system) strain from tensor **** (S system) [19]: **

, 2 2 2 2

{ } 33 11 22

2 2

33 12 13 23

( , ) cos sin sin sin

cos sin(2 ) sin cos sin(2 ) sin sin(2 )

*I L* *I* *I* *I*
*hkl* *i ij* *j*
*I* *I* *I* *I*
*m* *m*
ε φ ψ ε ε ε φ ψ ε φ ψ
ε ψ ε φ ψ ε φ ψ ε φ ψ
< > = = = +
+ + + + (2.40)

where: is strain tensor in the specimen system of reference, is the unit vector, in the
**direction of the scattering vector, expressed in the specimen system of reference (S). **

(2.41)
1 2
1 1
( )
2 2
*I* *I* *I* *I*
*ij* *Sijkl* *kl* *sijkl* *kl* *S* *ij* *kl* *S* *ik* *jl* *il* *jk* *kl*
ε = σ = σ =_{} δ δ + δ δ +δ δ _{}σ
*I*
*kl*
σ *I*
*ij*
ε
*ijkl*
*S* *sijkl*
*ij*
δ
,
{ } 33
( , ) *I L*
*hkl*
ε φ ψ ε
< > =
,
33
*I L*
ε *I*
*ij*
ε
*I*
*ij*
ε *m*
sin cos
sin sin
cos
*m*
ψ φ
ψ φ
ψ
=_{} _{}

31 Taking into consideration the Hook’s law (Eq. 2.1) and Eq. 2.40 it is possible to gain [19, 22]:

(2.42)

The above equation is a general expression relating first order mean stresses (full tensor) with strains measured for different directions of scattering vector described by

*ψ and ϕ angles and it is called sin2ψ law, because the measured strains are plotted vs. sin2ψ *

* (with constant ϕ). If the shear stresses are equal to zero, i.e. the sample system (S) *
coincides with principal axes of stress tensor, the latter plot is a straight line and the
components of the stress tensor can be extracted from the slope of the line plotted for

*constant ϕ.*

Usually a polycrystal is composed of elastically anisotropic crystallites (anisotropic
), stresses and strains vary over the differently oriented crystallites in the specimen as
a result of the elastic grain interaction [19]. Even then the whole specimen can be
macroscopically elastically isotropic (quasi-isotropic) when the crystallographic texture
does not occur and the grain interaction is isotropic. For quasi-isotropic specimens the
*S1 and 1/2S2 in Eq. 2.42 need to be replaced by hkl-dependent X-ray elastic constants *

*(XEC) S1hkl and 1/2S2hkl *[19], i.e.:

(2.43)

*In this case the XEC depends on the reflection hkl [23]. *

The most complex case is the textured polycrystalline material when macroscopic
elastic anisotropy is present. For such specimen the dependence of the X-ray-averaged
*strains on the mean stresses is described by the X-ray stress factors (XSF) Fij* depending

*not only on hkl but also on texture [1, 19, 24]: *

(2.44)

*where f represents ODF function. *

2 2 2

{ } 2 11 12 22

2

2 13 23 33 1 11 22 33

1

( , ) sin [ cos sin(2 ) sin ]

2 1

[ cos sin(2 ) sin sin(2 ) cos ] ( )

2
*I* *I* *I*
*hkl*
*I* *I* *I* *I* *I* *I*
*S*
*S* *S*
ε φ ψ ψ σ ϕ σ φ σ φ
σ φ ψ σ φ ψ σ ψ σ σ σ
< > = + + +
+ + + + + +
*ijkl*
*s*
2 2 2
{ } 2 11 12 22
2
2 13 23 33 1 11 22 33
1

( , ) sin [ cos sin(2 ) sin ]

2 1

[ cos sin(2 ) sin sin(2 ) cos ] ( )

2
*hkl* *I* *I* *I*
*hkl*
*hkl* *I* *I* *I* *hkl* *I* *I* *I*
*S*
*S* *S*
ε φ ψ ψ σ φ σ φ σ φ
σ φ ψ σ φ ψ σ ψ σ σ σ
< > = + + +
+ + + + + +
{ }
( , ) *hkl* *F hklij*( , , , )*f* *ijI*
ε φ ψ φ ψ σ
< > =

32

For textured materials or in the case of direction dependent grain interaction the
*sin2ψ plots are generally non-linear and the X-ray analysis can be challenging. The first *

works on stress analysis for sample having crystallographic texture were performed by Dole & Hauk (1978, 1979) [19].

*The X-ray elastic constants S1hkl and 1/2S2hkl* and the stress factors

can be evaluated experimentally by a uniaxial tension or bending test. It is also possible to calculate stress factors from single-crystal elastic constants using a model of crystallite coupling (Voigt, Reuss, Eshelby-Kröner) and the ODF as the weight function [1, 19]. Because the verification of used in grazing incident method is one of the aims of this work, the different models for calculation of these constants will be presented in next chapters.

It should be stated that using the diffraction methods, the lattice strain are not directly measured but in fact the interplanar spacings are determined from diffraction peak positions. These positions are measured for different orientations of the scattering vector with respect to the sample, defined by the φ and ψ angles. Using Eq. 2.44, after simple transformation the interplanar spacings can be expressed by the macrostresses

and stress free interplanar spacing:

(2.45)

or in the case of quasi-isotropic material:

(2.46)

The calculation of the stresses using Eqs. 2.45 or 2.46 can be performed using least square method and adjusting components of stress tensor as well as . However, the

whole stress tensor (principal stresses) can be calculated only if (stress free parameter) is known. Fortunately, in the case of X-ray diffraction penetrating thin surface layer (due to high absorption) we can assume that the forces normal to the surface are

( , , , )
*ij*
*F hkl* φ ψ *f*
( , , , )
*ij*
*F hkl* φ ψ *f*
{ }
( , ) *hkl*
*d* φ ψ
< >
*I*
*ij*
σ 0
}
*{hkl*
*d*
0 0
{ } , { } { }
*I*
*hkl* *ij* *ij* *hkl* *hkl*
*< d( ,*φ ψ *) _{>}*

*= [ F (hkl, ,*φ ψ

*f)*σ

*] d*+

*d*

### {

### }

### (

### )

2 2 2 11 33 12 22 33 0 0 { } 1 11 22 33 2 13 23 1( ) cos sin 2 ( ) sin

2 ( , )

1

( ) cos sin sin 2

2
*hkl* *I* *I* *I* *I* *I*
*hkl* *hkl* *hkl*
*hkl* *I* *I* *I* *hkl* *I* *I*
*S*
*d* *d* *d*
*S* *S*
σ σ φ σ φ σ σ ψ
ψ φ
σ σ σ σ φ σ φ ψ
− + + − +
< > = +
_{+} _{+} _{+} _{+} _{+}
0
}
*{hkl*
*d*
0
{*hkl*}
*d*

33 equal to zero and also =0. Because one of principal stresses is known, can be adjusted and its value can be also determined.

The least square procedure used in this work is based on minimising of the merit function called which is defined as:

(2.47)

where: and are the experimental and calculated

*interplanar spacings , δn=δn*( ) is the measurement error (standard

*deviation) of the determined spacing for the n-th measurement, N and M are the number of *
measured points and fitting parameters, respectively.

The value of χ² is a measure of goodness-of-fit, i.e. [25]:

• χ² = 1 means that the “good fit” was obtained (it corresponds to the fitting exactly within the limits of experimental uncertainty),

• *χ² < 1 the uncertainties of experimental data δn*( ) are overestimated,
• χ² > 1 the uncertainties of experimental data are underestimated or calculated

(theoretical) values *depending on stress factors Fij(hkl,ϕ ,ψ) are *

not accurate enough.

An example of stress calculation for the simplest case when elastic constants are isotropic (for tungsten) will presented in the next chapter when two standard methodologies are compared (Fig.3.6).

Finally it should be mentioned, that also the methods for determination of the second order stresses were developed using the elasto-plastic models [13, 14]. From these models the theoretical values of plastic incompatibility stresses ( - model values)

and the corresponding strains * can be predicted (where mod is used for the *
theoretical values). Assuming that stress variation with the ψ and angles is correctly
described by models, the measured strain can be expressed by the theoretical value, i.e.:

33
*I*
σ 0
}
*{hkl*
*d*
2
χ
( , ) *exp* ( , *cal* *2*
*N*
*n* *n* *{hkl}* *n* *n* *{hkl}*
*2*
*n 1* *n*
*d* *d*
*1*
* = *
*N* *M*
φ ψ φ ψ
χ
δ
=
_{<} _{>} _{− <} _{>}
−

### ∑

_{}

_{}( , )

*exp*

*n*

*n*

*{hkl}*

*d*φ ψ < > ( , )

*cal*

*n*

*n*

*{hkl}*

*d*φ ψ < > ( ,

_{n}*)*

_{n}*exp*

_{{hkl}}*d*φ ψ < > (

*,*

_{n}*)*

_{n}

_{{hkl}}exp*d*φ ψ < > (

*,*

_{n}*)*

_{n}*cal*

_{{hkl}}*d*φ ψ < > ,mod

*II*

*ij*σ ,mod { }

*II*

*hkl*

*< (*ε ψ φ

*, )>*φ

34

*; where: q - is a constant scaling factor. Finally, Eq. 2.45 *
takes form:

(2.48)

*When the value of q parameter is determined (as additional adjusting parameter) the plastic *
incompatibility stresses ( ) can be found for all grain orientations, i.e.: ;

where are the model predicted values. Thus, the macrostresses ( ) the mismatch

second order stresses ( ) can be determined simultaneously.

*2.3.2.DETERMINATION OF THIRD ORDER STRAINS AND CRYSTALLITE SIZE*

One of the features that decide about physical and mechanical properties of a solid body is its microstructure, such as lattice distortion or mosaic structure of grains. Using enough resolved diffractometers it is possible to observe the broadening of the diffraction peak due to the sample microstructure. The width of the diffraction peaks is also dependent on the size of the coherently diffracting domains, faulting on certain (hkl) planes, and microstrains within the coherently diffracting domains [26]. Peak broadening is further complicated by strain anisotropy, which can be taken into account by using contrast factor [27]. Not only sample but also instrument contribution convolute into the observed diffraction peak profile. Instrumental aberrations depend on the measuring technique and geometry. This effect can be taken into account by measuring a standard powder sample.

It is possible to separate the peak broadening originated from different causes. The broadening produced by small crystallite sizes and faulting is independent of the order of reflection, whereas the strain broadening depends on the order of reflection. Two methods are usually applied to separate these effects from each other [28].

The first, Warren and Averbach method (1950), based on the Fourier expansion of the intensity function and separation of size and strain series coefficients using diffraction peaks measured for at least two orders of reflection. The second is Williamson-Hall method (1953). It allows determine the domain size and the mean squared lattice strain by the analysis based on full width half maximum values or the integral breadths [28, 26].

,mod
{ } { }
*II*
*II*
*hkl* *hkl*
*< (*ε ψ φ*, ) _{>}*

*= q < (*ε ψ φ

*, )*,mod { } , { } { } { }

_{>}*I*

*II*

*hkl*

*ij*

*ij*

*hkl*

*o hkl*

*o hkl*

*< d(*ψ φ

*, )*

_{>}*= {*

_{F}*(hkl, ,*ψ φ

*f)*σ

*+ q < (*ε ψ φ

*, )*

_{>}*}*

_{d}*+*

_{d}

*II*

*ij*σ

*II*

*II*,mod

*ij = q*

*ij*σ σ ,mod

*II*

*ij*σ

*I*

*ij*σ

*II*

*ij*σ

35
It should be stated that the presented methods of analysis can be applied for crystallites
*having the size D < 100 nm and lattice distortions * grater than 10-3.

Warren and Averbach method

This method is based on the expansion of peak profile into Fourier series. In the case of X-ray diffraction (on laboratory apparatus) it is necessary to remove the influence of the Kα2 line from measured intensity. It can be done numerically with Rachinger

method [29] or analytically with the assumption of theoretical function describing the shape of the diffraction line [30] in which it is assumed that the intensity of line Kα2 is

twice smaller than the intensity of line Kα1 and both of the lines have the same shape and

the same width. Next, the effect of instrumental influence on the peak profile must be
taken into account using proposed by Stokes [31] harmonic analysis of diffraction line
profiles of the sample and reference sample and on the basis of them it is possible to obtain
*the actual intensity distribution function of the diffraction peak. The diffraction peak G(2θ) *
for reference is measured with the same conditions as this registered for the studied sample
*H(2θ). The latter profile can be expressed as the convolution of instrumental G(2θ) and *
*structural functions I(2θ): *

(2.49)

*If both functions G(2θ) and H(2θ) are expanded into Fourier series (the coefficients of such *
series are , and , ), the coefficients of the series given by Eqs. 2.26a and
2.26b can be calculated:

(2.50 a) and

(2.50 b)

where c is a constant factor.

*Finally the size of domain (D) in the direction of scattering vector and the square *
mean third order strain can be calculated applying Eqs. 2.26a, 2.26b and 2.27 for
peak intensities measured for two orders of reflections.

2
ε
< >
(2 ) ( ) (2 )
*H* θ *I* ϑ *G* θ ϑ ϑ*d*
∞
−∞
=

_{∫}

−
*n*

*g*

*g*'

_{n}*h*

_{n}*h*'

*2 2 ' ' ) ' )*

_{n}*n n*

*n*

*n*

*n*

*n*

*n*

*h*

*h*

*c*+ = +

*g*

*g*

*a*

*(g*

*(g*2 2 ' ' ) ' )

*n n*

*n n*

*n*

*n*

*n*

*h*

*h*

*c*− = +

*g*

*g'*

*a*

*(g*

*(g*2 ε < >